- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents
International Journal of Photoenergy
Volume 2013 (2013), Article ID 598753, 5 pages
Natural Dye-Sensitized Solar Cells Based on Highly Ordered TiO2 Nanotube Arrays
Key Laboratory of Ministry of Education for Advanced Materials in Tropical Island Resources, School of Materials and Chemical Engineering, Hainan University, Haikou 570228, China
Received 27 January 2013; Accepted 21 April 2013
Academic Editor: Theodoros Dimopoulos
Copyright © 2013 Na Li et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The dye-sensitized solar cells (DSSCs) have been fabricated using highly ordered TiO2 nanotube arrays as photoelectrode and natural dyes as photosensitizers. The natural dyes were extracted from the abundant plants in the tropical region, such as Tradescantia zebrina, kapok, and pitaya. The dyes could chemically couple with TiO2 nanotubes and effectively convert visible light into electricity in DSSCs. A power conversion efficiency could be achieved up to 0.3% in the solar cell sensitized by the extracts from kapok with a short-circuit current of 0.86 mA/cm2. Furthermore, the influences of the crystal structure of TiO2 nanotube arrays on the performance of the natural DSSCs were discussed.
Photosensitized wide-band gap metal-oxide semiconductors are used to convert visible light into electricity [1, 2]. In most dye-sensitized solar cells (DSSCs), nanocrystalline TiO2 films are used as photo-electrode due to their impressive properties when compared to other metal-oxide semiconductors. Most recently, different TiO2 nanostructures (nanotubes, nanorods, nanowires, nanoparticles, etc.) are explored as dye carriers [3–8]. Compared to other nanostructures, TiO2 nanotubes (TNTs) enhance much visible-light scattering and absorption due to their high length-to-diameter ratio and large surface area and facilitate electron transportation to the electrodes due to their unique geometry [9–12].
One of the key elements in DSSCs is photosensitizer. The most successful photo-induced electron transfer sensitizers employed so far in DSSCs are ruthenium (II) polypyridyl complexes. The ruthenium complexes in DSSCs have exhibited power conversion efficiencies up to 12% . Due to the high cost of ruthenium complexes and the scarce availability of those noble metals, looking for cheaper, simpler, and safer sensitizers becomes a scientific challenging problem . Natural pigments, including chlorophyll, anthocyanin, nasunin, and carotenoids, can fulfill those requirements, and sensitization of TiO2 by natural pigments has been reported [15–19]. Experimentally, natural dye-sensitized TiO2 solar cells have reached an efficiency of 7.1% .
Natural pigments extracted from leaves, flowers, and fruits of plants have advantages over rare metal complexes and other organic dyes. The natural dyes are readily available, easy to extract, of less cost, and environmentally friendly. In this work, we have made an attempt to collect red pigments from Tradescantia zebrina, kapok, and pitaya, as these plants are abundant in Hainan, the tropical island of China. The natural dyes were used to sensitize the highly ordered TiO2 nanotube arrays fabricated by chemical anodization technique. Then DSSCs were assembled, and the photoelectrical properties were investigated.
2.1. Preparation of Natural Dye-Sensitized TiO2 Solar Cells
Ti foils (0.5 mm thickness, 99.4% purity) were sequentially cleaned in acetone, ethanol, and deionized (DI) water. Anodization was then performed in a two-electrode configuration with titanium foil as the working electrode and a stainless steel foil as the counter electrode [11, 12, 20]. A direct current power supply was used as the voltage source to drive the anodization. The electrolyte consisted of 0.3 wt% NH4F and 2 vol% H2O in ethylene glycol. The anodization was conducted at 60 V for 2 h at room temperature. After anodization, the samples were annealed at 500°C or 600°C for 2 h in air with the temperature rising rate of 2°C/min.
All the fresh fruits and flowers were harvested in Hainan, the tropical island in China. The extracts of Tradescantia zebrina, kapok, and pitaya were obtained according to the similar steps as followed. The fresh fruits or flowers well cleaned (200 g) were crushed and soaked in 95% ethanol (50 mL) and then kept for 24 h in dark at room temperature. The residual parts were filtered. The clear solutions were centrifuged and diluted HCl was added to adjust the pH value. The solution with the extracts became red in color, and the natural dyes were ready to use as sensitizers in DSSCs.
TiO2 nanotube array electrodes were immersed at room temperature for 12 h in dark in the solution with the extracts, respectively. To evaluate the photovoltaic performance, TiO2 nanotube array electrode and Pt counter electrode were assembled to form a DSSC. The electrolyte was injected into the space between the two electrodes. The redox electrolyte with 1 : 9 was prepared by dissolving 0.5 M LiI and 0.05 M I2 in acetonitrile solution.
2.2. Characterization of Natural Dye-Sensitized TiO2 Solar Cells
The morphology and crystal structure of TiO2 nanotube-array electrode were characterized by field-emission scanning electronic microscopy (FESEM, Hitachi S4800, Japan) and X-ray diffraction technique (XRD, Bruker D8, Germany), respectively. The absorption spectrum of three kinds of natural extracts in solution and adsorbed onto TiO2 photoanode were measured by UV-visible absorption spectra measurements (Persee, TU-1901). Photocurrent-photovoltage characteristics of the natural dye-sensitized solar cells were measured by the electrochemical workstation (Zahner 6.0, Germany) with a xenon source with intensity of 50 mW/cm2. The effective cell area was 1.0 cm2.
3. Results and Discussion
3.1. Characteristics of TiO2 Nanotube-Array Electrode
Figure 1(a) shows the SEM image of the sample without ultrasonic treatment. The surface is covered with a layer of grassy residual and the nanotubes underneath are visible as shown in the inset of Figure 1(a). The grassy layer could block the infiltration of the dye and the redox electrolyte into the nanotubes. Thus it must be removed before the nanotubes are assembled into the DSSC . Ultrasonic treatment can remove the grassy layer and expose the underneath nanotubes, as shown in Figure 1(b). The nanotubes are well defined. As the nanotubular structure provides a high specific surface area, the nanotubes can absorb more dyes on the electrode surface as compared with the planar film.
Before being assembled into DSSCs, the samples were annealed for crystallization of the TiO2, since a large number of localized states in the amorphous structure without annealing can act as traps and recombination centers . Figure 2 shows the XRD patterns of TiO2 nanotubes annealed at different temperatures. It is evidenced that TiO2 transforms from amorphous phases to crystalline anatase phases and rutile phases after the annealing at 500°C. When the temperature increased to 600°C, the peaks relate to rutile phase increase.
3.2. Spectroscopic Characterization of Natural Photosensitizers
Figure 3(a) presents the absorption spectra of the red pigments in acid solutions, which were extracted from Tradescantia zebrina, kapok, and pitaya, respectively. The absorption peaks of the extracts from Tradescantia zebrina in visible-light region have maximums at 540 nm and 584 nm, which show typical absorption of anthocyanin . For the extracts from kapok in solution, the maximum of the absorption intensity in visible-light region is located at 406 nm and 508 nm, which correspond to the absorption of carotenoid [18, 23] and anthocyanin, respectively. And the absorption peak obtained for extracts from pitaya in visible-light region is at 400 nm. As shown in Figure 3(a), these red pigments in solution have maximum absorption peaks at 350 nm and 380 nm in ultraviolet region. The same locations of the absorption peaks mean that they contain similar compounds.
Figure 3(b) shows the absorption spectra of the extracts adsorbed on TiO2 electrodes, which were compared with that of TiO2 electrode without any dye sensitization. The bare TiO2 electrode cannot respond to the visible light due to its large band gap of 3.2 eV . However, a broad absorption peak in visible-light region extending from 380 to 680 nm was observed for the electrodes sensitized with the extracts of tradescantia zebriza, kapok, and pitaya. The natural dye sensitizers are thus found to effectively increase the absorption of the visible light, which dominates the terrestrial solar spectrum.
A close look at Figure 3 could found that the UV-vis absorption peaks of the dyes adsorbed on TiO2 electrodes are broadened and the peak positions are redshift, compared to those in solution. Such phenomenon can be explained as follows. Anthocyanin has a high absorption coefficient in the visible part of the solar spectrum. The binding between anthocyanin molecules and TiO2 semiconductor takes place through the carbonyl and hydroxyl groups. The chemical attachment could affect the energy levels of the highest occupied molecular level and the lowest unoccupied molecular level of the anthocyanidin molecules , which eventually affects the band gap and results in a shift of the absorption peak in the absorption spectra. Besides, the redshift of the visible-light absorption peaks could also be due to the complexation with metal ions .
3.3. Photoelectrochemical Performance of DSSCs Sensitized with Natural Dyes
Figure 4 shows the photocurrent-photovoltage (J-V) characteristics of the DSSCs. The photoelectrochemical parameters evaluated from Figure 4 are summarized in Table 1. The photoenergy conversion efficiencies () of the DSSCs sensitized with tradescantia zebriza, kapok, and pitaya are 0.23%, 0.3%, and 0.17%, respectively, and the short-circuit photocurrent densities are 0.63 mA/cm2, 0.87 mA/cm2, and 0.50 mA/cm2, respectively. The values of η and after natural dye sensitization are effectively enhanced in comparison to that without dye sensitization with the value of 0.006% and of 0.023 mA/cm2, while the open-circuit voltages and the fill factor are similar. This suggests that the chemical adsorption of the natural dye molecules on TiO2 electrodes takes place. The hydroxyl and carboxyl groups on anthocyanin are easy to chelate with Ti (IV) on TiO2 surface . This helps the excited electron quickly transfer from anthocyanin molecules to the conduction band of TiO2.
It can be seen from Table 1 that the DSSC sensitized with the extracts from kapok exhibits the best value of among the three kinds of dyes. This might be due to the higher intensity and broader range of the visible-light absorption of the extracts from kapok in comparison to the others as shown in Figure 3(b). Furthermore, stronger interaction between TiO2 and the dye molecules of the extracts of kapok also might lead to charge transfer quickly.
The stability of the natural dyes was further studied by continuous irradiation in the sunshine for 2 h and no significant changes were observed.
3.4. Effect of TiO2 Crystal Structure on the Performance of DSSCs
To further investigate the effect of TiO2 nanotube crystal structure on the natural DSSCs, characteristics of DSSCs at different annealing temperature were measured. As shown in Figure 5 and Table 2, the values of and for DSSCs based on TiO2 annealed at 500°C outperformed those annealed at 600°C. According to Figure 2, TiO2 nanotube arrays annealed at 500°C were major anatase phase with minor rutile ones. The electrode possesses the mixed crystal structure. When the temperature increased to 600°C, the sample has more obvious rutile peaks than the one annealed at 500°C. The results here suggest that the performance of DSSC based on TiO2 nanotube arrays depends on the proportion of anatase to rutile for TiO2 crystal structure. Besides the crystal structure, the geometric structure of TiO2 nanotube arrays can affect the photoelectrical properties and thus the performance of the DSSCs , which requires further experimental investigation.
The feasibility of assembling DSSCs with TiO2 nanotube arrays sensitized with three kinds of natural dyes has been demonstrated. Successful conversion of visible light into electricity was achieved. The efficiencies of the solar cells sensitized with the extracts of Tradescantia zebrine, kapok, and pitaya skin were up to 0.23%, 0.3%, and 0.17%, respectively. Crystalline phases of TiO2 significantly affect the photoenergy conversion parameters of DSSCs. Although our best values of DSSCs using kapok pigments are still lower than those obtained for the reference solar cells using the chemical dye N719, the simple extraction procedure, low cost, wide availability, and environmentally friendly nature make natural dyes as the promising sources of sensitizers for DSSCs. Through improving extraction method, refining natural dyes, and optimizing the geometric and crystal structures of TiO2 nanotube arrays, we believe that better results will be achieved.
This work was supported by Program for New Century Excellent Talents in University (NCET-09-0110), National Nature Science Foundation of China (51202050), Hainan Natural Science Foundation (511110), and Hainan University Youth Foundation (qnjj1241).
- B. O’Regan and M. Grätzel, “A low-cost, high-efficiency solar cell based on dye-sensitized colloidal TiO2 films,” Nature, vol. 353, no. 24, pp. 737–740, 1991.
- M. Grätzel, “Solar energy conversion by dye-sensitized photovoltaic cells,” Inorganic Chemistry, vol. 44, no. 20, pp. 6841–6851, 2005.
- J. R. Jennings, A. Ghicov, L. M. Peter, P. Schmuki, and A. B. Walker, “Dye-sensitized solar cells based on oriented TiO2 nanotube arrays: transport, trapping, and transfer of electrons,” Journal of the American Chemical Society, vol. 130, no. 40, pp. 13364–13372, 2008.
- A. Ghicov, S. P. Albu, R. Hahn et al., “TiO2 nanotubes in dye-sensitized solar cells: critical factors for the conversion efficiency,” Chemistry, vol. 4, no. 4, pp. 520–525, 2009.
- S. H. Kang, S. H. Choi, M. S. Kang, et al., “Nanorod-Based dye-sensitized solar cells with improved charge collection efficiency,” Advanced Materials, vol. 20, no. 1, pp. 54–58, 2008.
- J. Jiu, S. Isoda, F. Wang, and M. Adachi, “Dye-sensitized solar cells based on a single-crystalline TiO2 nanorod film,” The Journal of Physical Chemistry B, vol. 110, no. 5, pp. 2087–2092, 2006.
- B. Tan and Y. Wu, “Dye-sensitized solar cells based on anatase TiO2 nanoparticle/nanowire composites,” The Journal of Physical Chemistry B, vol. 110, no. 32, pp. 15932–15938, 2006.
- P. Roy, D. Kim, I. Paramasivam, and P. Schmuki, “Improved efficiency of TiO2 nanotubes in dye sensitized solar cells by decoration with TiO2 nanoparticles,” Electrochemistry Communications, vol. 11, no. 5, pp. 1001–1004, 2009.
- G. K. Mor, K. Shankar, M. Paulose, O. K. Varghese, and C. A. Grimes, “Use of highly-ordered TiO2 nanotube arrays in dye-sensitized solar cells,” Nano Letters, vol. 6, no. 2, pp. 215–218, 2006.
- K. Zhu, N. R. Neale, A. Miedaner, and A. J. Frank, “Enhanced charge-collection efficiencies and light scattering in dye-sensitized solar cells using oriented TiO2 nanotubes arrays,” Nano Letters, vol. 7, no. 1, pp. 69–74, 2007.
- D. H. Li, S. W. Lin, S. P. Li, et al., “Effects of geometric and crystal structures on the photoelectrical properties of highly-ordered TiO2 nanotube arrays,” Journal of Materials Research, vol. 27, no. 7, pp. 1029–1036, 2012.
- S. P. Li, S. W. Lin, J. J. Liao, et al., “Nitrogen-doped TiO2 nanotube arrays with enhanced photoelectrochemical property,” International Journal of Photoenergy, vol. 2012, Article ID 794207, 7 pages, 2012.
- A. Yella, H. W. Lee, H. N. Tsao, et al., “Porphyrin-sensitized solar cells with cobalt (II/III)-based redox electrolyte exceed 12 percent efficiency,” Science, vol. 334, no. 6056, pp. 629–634, 2011.
- W. M. Campbell, A. K. Burrell, D. L. Officer, and K. W. Jolley, “Porphyrins as light harvesters in the dye-sensitised TiO2 solar cell,” Coordination Chemistry Reviews, vol. 248, no. 13-14, pp. 1363–1379, 2004.
- N. J. Cherepy, G. P. Smestad, M. Grätzel, and J. Z. Zhang, “Ultrafast electron injection: implications for a photoelectrochemical cell utilizing an anthocyanin dye-sensitized TiO2 nanocrystalline electrode,” The Journal of Physical Chemistry B, vol. 101, no. 45, pp. 9342–9351, 1997.
- K. Wongcharee, V. Meeyoo, and S. Chavadej, “Dye-sensitized solar cell using natural dyes extracted from rosella and blue pea flowers,” Solar Energy Materials and Solar Cells, vol. 91, no. 7, pp. 566–571, 2007.
- G. Calogero and G. D. Marco, “Red Sicilian orange and purple eggplant fruits as natural sensitizers for dye-sensitized solar cells,” Solar Energy Materials and Solar Cells, vol. 92, no. 11, pp. 1341–1346, 2008.
- E. Yamazaki, M. Murayama, N. Nishikawa, N. Hashimoto, M. Shoyama, and O. Kurita, “Utilization of natural carotenoids as photosensitizers for dye-sensitized solar cells,” Solar Energy, vol. 81, no. 4, pp. 512–516, 2007.
- Q. Dai and J. Rabani, “Photosensitization of nanocrystalline TiO2 films by pomegranate pigments with unusually high efficiency in aqueous medium,” Chemical Communications, no. 20, pp. 2142–2143, 2001.
- H. Omidvar, S. Goodarzi, A. Seif, and A. R. Azadmehr, “Influence of anodization parameters on the morphology of TiO2 nanotube arrays,” Superlattices and Microstructures, vol. 50, no. 1, pp. 26–39, 2011.
- A. Ghicov and P. Schmuki, “Self-ordering electrochemistry: a review on growth and functionality of TiO2 nanotubes and other self-aligned MOx structures,” Chemical Communications, no. 20, pp. 2791–2808, 2009.
- Q. Dai and J. Rabani, “Photosensitization of nanocrystalline TiO2 films by anthocyanin dyes,” Journal of Photochemistry and Photobiology A: Chemistry, vol. 148, no. 1–3, pp. 17–24, 2002.
- F. G. Gao, A. J. Bard, and L. D. Kispert, “Photocurrent generated on a carotenoid-sensitized TiO2 nanocrystalline mesoporous electrode,” Journal of Photochemistry and Photobiology A: Chemistry, vol. 130, no. 1, pp. 49–56, 2000.
- M. Grätzel, “Perspectives for dye-sensitized nanocrystalline solar cells,” Progress in Photovoltaics: Research and Applications, vol. 8, no. 1, pp. 171–185, 2000.
- S. Meng, J. Ren, and E. Kaxiras, “Natural dyes adsorbed on TiO2 nanowire for photovoltaic applications: enhanced light absorption and ultrafast electron injection,” Nano Letters, vol. 8, no. 10, pp. 3266–3272, 2008.